InÀuence of Serum Supplemented Cell Culture Medium on Colloidal
Stability of Polymer Coated Iron Oxide and Polystyrene Nanoparticles
With Impact on Cell Interactions In Vitro
Vera Hirsch , Jatuporn Salaklang , Barbara Rothen-Rutishauser , and Alke Petri-FinkAdolphe Merkle Institute, 1723 Marly 1, Switzerland
University of Fribourg, Department of Chemistry, 1700 Fribourg, Switzerland Respiratory Medicine, Bern University Hospital, Inselspital, Bern 3010Switzerland
When nanoparticles interact with cells, the possible cellular responses to the particles depend on an array of parameters, in both particle and biological aspects. On the one hand, the physicochemical properties of the particles (e.g., material, size, shape, and surface charge) are known to play a key role in particle-cell interactions. On the other hand, it has been shown that prior to coming into contact with cells, nanoparticle interaction with the surrounding biological Àuid may lead to a change of the initial particle properties. For example, the colloidal behavior of nanoparticles is strongly inÀuenced by the density and viscosity of the surrounding media in both in
vitro and in vivo systems.
In this study, we demonstrate how the surface charge and composition of different nanoparticles can impact upon their physicochem-ical characteristics, such as their colloidal stability, within a representative biologphysicochem-ical Àuid and how the change of these parameters can signi¿cantly inÀuence the subsequent cellular interaction in vitro. Therefore, we compared charged polymer coated superparamagnetic iron oxide nanoparticles to polystyrene nanoparticles of different surface charges. Particles of lower colloidal stability, namely positively charged superparamagnetic iron oxide nanoparticles, and the polystyrene nanoparticles, showed a higher cell-penetration in vitro than the colloidally stable particles.
WITH the rapidly progressing development of
nano-based materials and applications in the past decade , the interactions of nanoparticles (NPs) with biolog-ical systems has gained increased attention within the ¿eld of nanoscience –.
Cellular responses to NPs depend on an array of different intrinsic properties of the particle in question (e.g., material, size, shape, and surface charge) –. The particle’s surface charge (i.e., the functional surface groups) plays a key role in particle-cell interaction ,  by direct interaction with the outer cell membrane . In addition, the surface charge of NPs strongly impacts upon their colloidal behaviour .
Before particles interact with cells, their intrinsic physico-chemical properties may change due to interaction with the pro-teins (e.g., blood serum propro-teins) and electrolytes present within the surrounding biological Àuid , . This possible change of the initial properties of the particle can lead to the aggrega-tion of NPs, which may cause unexpected results in the assess-ment of in vitro and in vivo experiassess-ments , . The pos-sible higher sedimentation velocity of NP-aggregates within in
vitro cultures for example can promote a higher concentration
of NPs on the outer cell membrane, resulting in a mistaken ob-servation of increased cell uptake , , since cell uptake is directly linked with the concentration of present particles .
Corresponding author: A. Petri-Fink (e-mail: alke.¿firstname.lastname@example.org).
Therefore, it is of highest importance to ¿rst understand how NPs interact with their surrounding biological media, before in-vestigating and interpreting responses and effects of NPs at a cellular or in vivo level.
The use of superparamagnetic iron oxide nanoparticles (SPIONs) in both biomedical research and clinical applications has increased signi¿cantly in the last decade ,  as they represent useful tools for magnetic separation purposes (e.g., rapid DNA sequencing)  and can be used as contrast en-hancers in the ¿eld of magnetic resonance imaging –. Polystyrene NPs have demonstrated a low cytotoxicity pro¿le and are widely used as biocompatible model drug carrier systems for in vitro and in vivo experiments –.
The aim of the paper is to determine how different surface charges (i.e., different functional surface groups) and different particle composition (i.e., iron oxide versus polystyrene) may impact upon the intrinsic physicochemical properties of these NPs, such as their colloidal stability, within a representative bi-ological Àuid (i.e., fetal bovine serum supplemented cell culture medium) and how this may affect the subsequent cellular uptake
A. Chemicals and Reagents
All chemicals were purchased from Sigma Aldrich, Switzer-land unless otherwise stated and were of analytical reagent grade and used without further puri¿cation. Water refers in all synthesis steps to ultrapure deionized water of 18
(Millipore AG, Switzerland). The serum was EU approved fetal bovine serum (FBS) originating from a singular batch (refer-ence n 10270106, lot n 41G8582K, Invitrogen, Switzerland).
Published in ",(((7UDQVDFWLRQVRQ0DJQHWLFV" which should be cited to refer to this work.
B. PVA Coated SPIONs
Superparamagnetic iron ixide nanoparticles (SPIONs) were prepared by alkaline coprecipitation of ferric and ferrous chlo-rides in aqueous solution as described previously – and characterized thoroughly by X-ray diffraction (XRD), surface area measurements (Brunner, Emmet, and Teller (BET) method) and magnetic measurements as previously described by Chastellain et al. . The uncoated SPIONs were subsequently coated with polyvinyl alcohol (PVA), viny-lalcohol/vinylamine copolymer or carboxylated PVA (i.e., PVA with randomly distributed carboxylic acid groups) in order to obtain different charged surfaces . The PVA had an average molecular weight (MW) of 14 000 g/mol and a hydrolysis degree of 83% and was supplied by Omya AG, Switzerland (Mowiol 3-83). Vinylalcohol/Vinylamine copolymer, with an average MW of 80 000–140 000 was supplied by Erkol S.A, Spain (M12) and carboxyl-modi¿ed PVA was supplied by Ku-raray Specialties Europe GmbH, Germany (KL506). Polymer solutions (10% w/v Mowiol 3-83, 2% w/v M12, and 6% w/v KL506) were added to the NP suspensions in a v/v ratio of one and the pH of the ¿nal suspensions was adjusted to seven using a 5% aqueous ammonia solution. The particles will be referred to as OH-PVA-SPIONs (i.e., regular PVA-SPIONs)
and -PVA-SPIONs and COOH-PVA-SPIONs (i.e.,
func-tionalized PVA-SPIONs) in this work.
Hydroxyl-, amino-, and carboxyl-modi¿ed polystyrene nanoparticles (PS-NPs) were purchased from Merck (Merck, Switzerland). Detailed characterization of the purchased nanoparticles has been carried out in-house by photon corre-lation spectroscopy (PCS). The particles will be referred to as
OH-PS-NPs, -PS-NPs and COOH-PS-NPs in this work.
D. Iron Quanti¿cation
Uncoated SPIONs were quanti¿ed by (i) titration with potassium permanganate, as previously described by Skoog . Polymer coated particles were then quanti¿ed using the Prussian blue colorimetric assay ( served as the negative control) by dissolving the particles in 6 N HCl (Honeywell
Burdick, and Jackson) (50 of a 96-well plate) for
one hour. Subsequently, 50 of a freshly prepared 5% (Merck, Switzerland) solution was added to each well. The absorbance was then determined at a wavelength of 690 nm using a multi-label plate reader ( , PerkinElmer,
Switzerland) . The standard curve was established
using previously analyzed uncoated SPIONs.
E. PS Quanti¿cation
Polystyrene shows an absorbance maximum at 259 nm when dissolved in an organic solvent. In addition, polystyrene solu-tions are also Àuorescent. To determine the concentration of the NP suspension, the amount of PS present in the uncoated PS-NP suspension was measured following the method described by Muller and Schuber . BrieÀy, PS-NPs were dissolved in Dimethoxyethane (DME, Sigma Aldrich, Switzerland) and Àu-orescence was measured after 10 min at 335 nm in a range of 2–10 ( served as the negative control) in a 96-well quartz plate (TECAN, Switzerland). Each experiment was
per-formed in triplicate .
F. Particle Characterization by Photon Correlation Spectroscopy (PCS)
The physicochemical parameters of the different uncoated and coated NPs, speci¿cally the size and zeta potential, were assessed via light-scattering measurements at 90 by PCS equipped with a BI-9000AT digital autocorrelator (Brookhaven Instruments Cooperation, LABORCHEMIE GmbH, Austria). The CONTIN method was used for data processing. The NP suspensions were diluted in 20 mM borate buffer (pH 7.5) to perform the measurements. Viscosity, refractive index and dielectric constant of pure water were used to characterize the solvent.
G. Cell Culture
Human cervix carcinoma cells (HeLa cells) were purchased from HPA Culture Collections UK and cultured in at 75
cell culture Àask at 37 and 5% . Dulbecco’s
Modi-¿ed Eagle Medium 1 (DMEM phenol red free, Invitrogen, Switzerland) supplemented with 10% fetal bovine serum and 1% Penicillin/Streptomycin (Invitrogen, Switzerland) was used throughout all the experiments. At 24 h prior to experimen-tation cells were detached using Trypsin-EDTA (Invitrogen, Switzerland) and their viability was determined via Trypan blue exclusion. In a 48 well-plate (Costar, Corning Incorporated,
USA), HeLa cells were seeded at a density of cells
per well and were cultured at 37 and 5% for 24 h prior to NP exposure.
H. NP Exposure
Prior to NP exposure cells were washed with PBS. The in-vestigated NPs were added at a concentration of 100
of iron or PS in 10% FBS supplemented cell culture medium and incubated for 1, 6, and 24 h at 37 and 5% . Supple-mented cell culture medium, in the absence of particles, acted as the negative control.
I. Cell Uptake Determination by Cellular Iron Quanti¿cation
The ability of each PVA-SPION type to enter HeLa cells after 1, 6, and 24 h of exposure at 100 iron/mL was determined using the Prussian Blue assay as previously described. BrieÀy, after exposure to PVA-SPIONs the cell layer was dissolved in 6 N HCl (100 of a 48-well plate) for 1 h, then 50
of a 5% aqueous solution of (Merck, Switzerland)
was added and the absorbance was measured at 690 nm using a multilabel plate reader ( , PerkinElmer, Switzerland) after 10 min. A standard curve of the differently coated SPIONs was recorded to quantify the mass of cell internalized iron. The iron content in cells not exposed to SPIONs was always below the detection limit of 1 ppm. Each experiment was performed in
J. Lactate Dehydrogenase (LDH) Release
A Cytotoxicity Detection Kit (Roche Applied Science, Ger-many) was used to quantify the level of cytotoxicity exerted upon the HeLa cells after exposure to PVA-SPIONs. This calori-metric assay is based on the measurement of LDH activity, an enzyme released from the cytosol of damaged cells into the su-pernatant. Hela cells were cultured as described above.
COOH-PVA-SPIONs, -PVA-SPIONs and OH-PVA-SPIONs were
exposed to HeLa cells in 10% FBS supplemented cell culture
media at 100 iron for 24 h at 37 and 5% . The negative control was 10% FBS-supplemented cell culture media alone. The detergent Triton X-100 acted as the positive con-trol at a concentration of 0.2% in PBS. Each exposure was re-peated a total of four times . Supernatants were mea-sured in triplicate at 490 nm (with a reference of 630 nm) using a multi-plate spectrometer (Benchmark Plus, Bio-Rad, Switzer-land). Total extracellular LDH was then measured according to the manufacturer’s manual.
K. Cell Uptake Determination by Fluorescence Spectroscopy
HeLa cell uptake of the different PS-NPs was determined using the method described above. BrieÀy, after exposure of 100 PS/mL, for 1, 6, and 24 h, the cell layer was mechan-ically destroyed by repeated pipetting (after the addition of 100 water/well in a 48-well plate). Then an equal volume of Dimethoxyethane (DME, Sigma Aldrich, Switzerland) was added and Àuorescence was measured after 10 min at 335 nm. Each experiment was performed in triplicate .
L. Turbidity Measurements by UV/Vis-Spectroscopy
Turbidity measurements of all NPs were carried out by mixing the suspensions (100 ) with the cell culture medium in the presence of 10% FBS. After rapid homoge-nization by gently pipetting the suspension up and down, the turbidity was measured at 480 nm (PVA-SPIONs) and 556 nm (PS-NPs) over 24 h in special optical glass precision cells from Hellma Analytics (Hellma GmbH & Company KG). All results were normalized against supplemented cell culture medium alone and each experiment was performed in triplicates
III. RESULTS ANDDISCUSSION
A. Characterization of Nanoparticles
After synthesis, the uncoated SPIONs showed a mean diam-eter (d50) of 11.9 3.7 nm as obtained by dynamic light scat-tering (DLS) and a positive zeta potential of 34.6 1.6 mV . Subsequent polymer coating led to an increased d50
of 34.9 7.2 nm and zeta potentials of , 29.4
1.3 mV and 1.5 2.3 mV for COOH-PVA-SPIONs,
-PVA-SPIONs and OH-PVA-SPIONs, respectively. Hydroxyl-, amino- and carboxyl-modi¿ed polystyrene nanoparticles (PS-NPs) were purchased from Merck (Merck, Switzerland). DLS showed a d50 of 63.9 7.0 nm, 83.3
8.0 nm and 76.67 4.6 nm and a zeta potential of
, 8.8 1.4 mV and 2.6 4.1 mV for
COOH-PS-NPs, -PS-NPs and OH-PS-NPs, respectively. Both particle types, i.e., PS-NPs and SPIONs, showed com-parable sizes whereas their zeta potentials varied according to their functional surface groups (Table I).
All NPs were stable in ultra-pure water and phosphate buffer over months (data not shown).
B. Nanoparticle-Cell Interactions
To study the importance of surface charges and consequently the impact of functional surface groups and composition of the NPs on the subsequent cellular interaction, HeLa cells were ex-posed in cell culture medium supplemented with 10% FBS to 100 of iron (for the different PVA coated iron oxide
MEANPARTICLESIZE ANDZETAPOTENTIAL FORPVA-SPIONS ANDPS-NPS
Fig. 1. Cell uptake of the different investigated PVA-SPIONs. The amount of cell uptake is shown as % of total added iron as a function of incubation time after NP exposure at a concentration of 100 iron/mL to HeLa cells in 10%
FBS supplemented cell culture medium ( , ).
Fig. 2. Cell uptake of the different investigated PS-NPs. The amount of cell uptake is shown as % of total added PS as a function of incubation time after NP exposure at a concentration of 100 PS/mL HeLa cells in 10% FBS
sup-plemented cell culture medium ( , ).
nanoparticles) or 100 of PS (in case of the PS-NPs) for 1, 6, and 24 h. All data is presented in quantities of mass of iron/mL suspension (instead of polymer coated SPIONs) to allow comparison with the common literature. The uptake of the particles was measured by quanti¿cation of the intracellular iron and PS content by assessing the Prussian Blue reaction for SPIONs (Fig. 1) and the described Àuorescence assay for PS-NPs (Fig. 2). The reliability of the Prussian blue reaction for the quanti¿cation of intracellular iron in vitro has been re-ported previously . The intracellular iron content of cells not exposed to any of the studied PVA-SPIONs was constantly below the detection limit of one ppm. The Àuorescence assay was adapted from Muller and Schuber, who developed a sensi-tive method for the quanti¿cation of polystyrene latex beads by measuring the intrinsic Àuorescence of polystyrene dissolved in organic solvents .
Figs. 1 and 2 show that cell uptake of -functionalized PVA-SPIONs (i.e., positively charged PVA-SPIONs) by HeLa cells was higher than the cell uptake of OH- or COOH-PVA-SPIONs (i.e., neutral and negatively charged PVA-COOH-PVA-SPIONs). Furthermore, cell uptake of -PVA-SPIONs increased over
Fig. 3. Release of lactate dehydrogenase (LDH) in % relative to Triton X-100. COOH-PVA-SPIONs, OH-PVA-SPIONs and -PVA-SPIONs were ex-posed to HeLa cells at 100 iron in 10% FBS supplemented cell culture media for 24 h. Triton X-100 acted as the positive control at a concentration of 0.2% in PBS. The negative control was 10% FBS supplemented cell culture
media only ( ; ).
Fig. 4. Stability of all investigated PVA-SPIONs. The stability of NPs is pre-sented as UV/Vis absorbance at 480 nm as a function of incubation time after NP incubation of 100 iron/mL in 10% FBS supplemented cell culture medium
( , ).
time, whereas cell uptake stayed constantly low for OH- and COOH-PVA-SPIONs. Compared to this, a relatively high cell uptake was observed for all PS-NP types within the ¿rst hour and the internalization of these NPs increased equally over time. It has been previously reported that uncoated iron oxide NPs could have toxic effects on cells . However, the outer polymer coating layer covering the SPIONs has a greater inÀu-ence on the cytotoxicity of polymer coated NPs than the core SPIONs themselves , . In previous studies, we have already investigated the cytotoxicity of PVA-SPIONs using the MTT assay . No cytotoxicity in HeLa cells was observed for the PVA-SPIONs over a 24 h period up to 100 iron/mL using the LDH assay and measuring the release of the cytosolic enzyme lactate dehydrogenase (Fig. 3)
C. Turbidity Measurements by UV/Vis-Spectroscopy
The colloidal behavior of NPs suspended in biological Àuids i.e., the size of potential aggregates, impacts signi¿cantly upon any cellular and biological effects both in vitro and in vivo , , , .
In this study, the agglomeration behavior of the NPs was es-timated by turbidity measurements (Figs. 3 and 4) which, in contrast to the exact determination of particle sizes, is straight-forward and easily reproducible .
Fig. 3 shows that compared to the OH- and COOH-PVA-SPIONs only the -functionalized PVA-SPIONs tend to gregate in serum-supplemented cell culture medium and that ag-gregation progresses over time. Fig. 4 shows that in the tested biological Àuid all three investigated PS-NP aggregated within the ¿rst hour and aggregation remained constant over a 24 h pe-riod. All investigated NPs were stable in water for more than a
Fig. 5. Stability of all investigated PS-NPs. The stability of NPs is presented as UV/Vis absorbance at 566 nm as a function of incubation time after NP incuba-tion of 100 PS/mL in 10% FBS supplemented cell culture medium ( ,
month at pH 2 and pH 7 without showing any signs of agglom-eration (data not shown).
The observation that colloidally less stable NPs showed a higher cell uptake compared to colloidally stable NPs could be due to the possibility that larger NPs or aggregates elicit a higher sedimentation velocity within in vitro cultures and thus lead to a higher particle concentration on the cell surface, resulting in a misrepresentative increased cell uptake , , since cell uptake is directly linked to the concentration of present particles .
The preferred uptake of aggregated NPs might also be ex-plained by the speci¿c uptake mechanism of HeLa cells . Although epithelial cells are known to have a rather low phago-cytic rate compared to other cells (i.e., phagophago-cytic cells like macrophages), Stone et al. showed that epithelial cells can use this active mechanism for uptake of NPs . Investigating the impact of size of receptor-targeting transferrin-coated gold NP aggregates on their cellular uptake and subsequent biological impact on epithelial cells (i.e., HeLa and A549 cells) and car-cinoma cells (i.e., MDA-MB-435 cells), Albanese and Chan showed that, depending on the type of cell, an array of cellular responses to NP aggregates are possible . It is well recog-nized that the cellular responses to materials at the nanoscale generally depend on the cell type, a phenomenon which is usu-ally described as cell “Vision” .
In this study, we compared the impact of different surface charges (i.e., different functional surface groups) and different particle compositions (i.e., iron oxide versus polystyrene) on colloidal stability and subsequent cellular interaction in vitro. After exposure to HeLa cells, in the presence of serum-sup-plemented cell culture medium, cell uptake of positively charged PVA-SPIONs (i.e., PVA-SPIONs bearing -groups on the surface) was signi¿cantly faster and higher compared to both neutral and negatively charged PVA-SPIONs (i.e., PVA-SPIONs bearing OH- and COOH-groups on the surface). PS-NPs showed a comparably high cell uptake independent of their surface charge. Turbidity measurements showed that pos-itively charged PVA-SPIONs in turn showed a lower colloidal stability than neutral and negatively charged PVA-SPIONs. For PS-NPs, a generally low colloidal stability was observed. Here we showed that cell uptake can be independent of NP-composition (i.e., core and/or coating material), and that it strongly depends on the physicochemical changes that NPs
may undergo in biological Àuids. The possible alteration of the physicochemical characteristics of the NPs in turn impacts upon their colloidal stability and consequently on their cellular uptake.
In-depth light scattering and stereological investigations will reveal the size and polydispersity of the occurring aggregates in supplemented cell culture medium and inside the cells. This will help understand the impact of aggregation on subsequent cellular uptake in a quantitative way. Cho et al., studied the sedimentation/diffusion velocity ratio, with respect to enhanced cellular uptake, and de¿ned a critical ratio of three . How-ever, due to the comparably low density of the NPs used in this study, sedimentation cannot be the only reason to explain the much-increased cellular uptake. Consequently, colloidal prop-erties should be investigated in more detail to better correlate cellular and material data.
This work was supported in part by the Swiss National Science Foundation (PP00P2-123373/1), the Adolphe Merkle Foundation, the University of Fribourg, and by the Fribourg Center for Nanomaterials (FriMat). The authors acknowledge Dr. B. D. Johnston for proofreading the manuscript.
The authors declare no conÀicts of interest. The authors are entirely responsible for the writing of the manuscript and for the content presented within it.
 K. Riehemann, S. W. Schneider, T. A. Luger, B. Godin, M. Ferrari, and H. Fuchs, “Nanomedicine—Challenge and perspectives,” Angew.
Chem. Int. Ed. Engl, vol. 48, no. 5, pp. 872–897, 2009.
 M. Beija, R. Salvayre, N. Lauth-de Viguerie, and J.-D. Marty, “Col-loidal systems for drug delivery: From design to therapy,” Trends in
Biotechnol., vol. 30, no. 9, p. 485, 2012.
 K. Donaldson, “Nanotoxicology,” Occupational Environ. Med., vol. 61, no. 9, pp. 727–728, 2004.
 G. Oberdörster, E. Oberdörster, and J. Oberdörster, “Nanotoxicology: An emerging discipline evolving from studies of ultra¿ne particles,”
Environ. Health Perspect., vol. 113, no. 7, pp. 823–839, 2005.
 S. K. Sohaebuddin, P. T. Thevenot, D. Baker, J. W. Eaton, and L. Tang, “Nanomaterial cytotoxicity is composition, size, and cell type depen-dent,” Part Fibre Toxicol., vol. 7, no. 1, p. 22, 2010.
 W. Jiang, B. Y. S. Kim, J. T. Rutka, and W. C. W. Chan, “Nanoparticle-mediated cellular response is size-dependent,” Nature Nanotechnol., vol. 3, no. 3, pp. 145–150, 2008.
 E. C. Cho, J. Xie, P. A. Wurm, and Y. Xia, “Understanding the role of surface charges in cellular adsorption versus internalization by se-lectively removing gold nanoparticles on the cell surface with a I 2/KI etchant,” Nano Lett., vol. 9, no. 3, pp. 1080–1084, 2009.
 E. C. Cho, L. Au, Q. Zhang, and Y. Xia, “The effects of size, shape, and surface functional group of gold nanostructures on their adsorption and internalization by cells,” Small, vol. 6, no. 4, pp. 517–522, 2010.  A. Verma and F. Stellacci, “Effect of surface properties on
nanopar-ticle—Cell interactions,” Small, vol. 6, no. 1, pp. 12–21, 2010.  K. Unfried, C. Albrecht, L.-O. Klotz, A. von Mikecz, S. Grether-Beck,
and R. P. Schins, “Cellular responses to nanoparticles: Target structures and mechanisms,” Nanotoxicology, vol. 1, no. 1, pp. 52–71, 2007.  A. Petri-Fink, M. Chastellain, L. Juillerat-Jeanneret, A. Ferrari, and
H. Hofmann, “Development of functionalized superparamagnetic iron oxide nanoparticles for interaction with human cancer cells,”
Bioma-terials, vol. 26, no. 15, pp. 2685–2694, 2005.
 C. C. Fleck and R. R. Netz, “Electrostatic colloid-membrane binding,”
Europhys. Lett, vol. 67, no. 2, pp. 314–320, 2004.
 J. Adair, E. Suvaci, and J. Sindel, “Surface and colloid chemistry of advanced ceramics,” in Encyclopedia of Materials: Science and
Tech-nology. Amsterdam, The Netherlands: Elsevier, pp. 8996–9006.
 R. C. Murdock, L. Braydich-Stolle, A. M. Schrand, J. J. Schlager, and S. M. Hussain, “Characterization of nanomaterial dispersion in solution prior to in vitro exposure using dynamic light scattering technique,”
Toxicol. Sci., vol. 101, no. 2, pp. 239–253, 2008.
 D. B. Warheit, “How meaningful are the results of nanotoxicity studies in the absence of adequate material characterization?,” Toxicol. Sci., vol. 101, no. 2, pp. 183–185, 2008.
 K. Rausch, A. Reuter, K. Fischer, and M. Schmidt, “Evaluation of nanoparticle aggregation in human blood serum,” Biomacromolecules, vol. 11, no. 11, pp. 2836–2839, 2010.
 G. Maiorano, S. Sabella, B. Sorce, V. Brunetti, M. A. Malvindi, R. Cin-golani, and P. P. Pompa, “Effects of cell culture media on the dynamic formation of protein-nanoparticle complexes and inÀuence on the cel-lular response,” ACS Nano, vol. 4, no. 12, pp. 7481–7491, 2010.  J. G. Teeguarden, P. M. Hinderliter, G. Orr, B. D. Thrall, and J. G.
Pounds, “Particokinetics in vitro: Dosimetry considerations for in vitro nanoparticle toxicity assessments,” Toxicol. Sci., vol. 95, no. 2, pp. 300–312, 2006.
 E. C. Cho, Q. Zhang, and Y. Xia, “The effect of sedimentation and dif-fusion on cellular uptake of gold nanoparticles,” Nature Nanotechnol., vol. 6, no. 6, pp. 385–391, 2011.
 C. Xu, G. A. Tung, and S. Sun, “Size and concentration effect of gold nanoparticles on x-ray attenuation as measured on computed tomog-raphy,” Chem. Mater., vol. 20, no. 13, pp. 4167–4169, 2008.  M. Mahmoudi, H. Hofmann, B. Rothen-Rutishauser, and A. Petri-Fink,
“Assessing the in vitro and in vivo toxicity of superparamagnetic iron oxide nanoparticles,” Chem. Rev., vol. 112, no. 4, pp. 2323–2338, 2012.  S. Laurent, D. Forge, M. Port, A. Roch, C. Robic, L. Vander Elst, and R. N. Muller, “Magnetic iron oxide nanoparticles: Synthesis, stabiliza-tion, vectorizastabiliza-tion, physicochemical characterizations, and biological applications,” Chem. Rev., vol. 108, no. 6, pp. 2064–2110, 2008.  Q. A. Pankhurst, J. Connolly, S. K. Jones, and J. Dobson, “Applications
of magnetic nanoparticles in biomedicine,” J. Phys. D: Appl. Phys., vol. 36, no. 13, p. R167, 2003.
 A. Petri-Fink and H. Hofmann, “Superparamagnetic iron oxide nanoparticles (SPIONs): From synthesis to in vivo studies—A summary of the synthesis, characterization, in vitro, and in vivo in-vestigations of SPIONs with particular focus on surface and colloidal properties,” IEEE Trans. Nanobiosci., vol. 6, no. 4, pp. 289–297, Dec. 2007.
 C. Sun, J. Lee, and M. Zhang, “Magnetic nanoparticles in MR imaging and drug delivery,” Adv. Drug Del. Rev., vol. 60, no. 11, pp. 1252–1265, 2008.
 L. Frullano and T. J. Meade, “Multimodal MRI contrast agents,” JBIC
J. Biol. Inorganic Chem., vol. 12, no. 7, pp. 939–949, 2007.
 C. Corot, P. Robert, J. Idee, and M. Port, “Recent advances in iron oxide nanocrystal technology for medical imaging,” Adv. Drug Del.
Rev., vol. 58, no. 14, pp. 1471–1504, 2006.
 P. Menei, A. Croué, V. Daniel, A. Pouplard-Barthelaix, and J. P. Benoit, “Fate and biocompatibility of three types of microspheres implanted into the brain,” J. Biomed. Mater. Res., vol. 28, no. 9, pp. 1079–1085, 1994.
 P. Jani, G. W. Halbert, J. Langridge, and A. T. Florence, “The up-take and translocation of latex nanospheres and microspheres after oral administration to rats,” J. Pharm. Pharmacol., vol. 41, no. 12, pp. 809–812, 1989.
 T. Blunk, D. F. Hochstrasser, J. C. Sanchez, B. W. Müller, and R. H. Müller, “Colloidal carriers for intravenous drug targeting: Plasma protein adsorption patterns on surface-modi¿ed latex particles eval-uated by two-dimensional polyacrylamide gel electrophoresis,”
Elec-trophoresis, vol. 14, no. 12, pp. 1382–1387, 1993.
 M. Chastellain, A. Petri, and H. Hofmann, “Particle size investigations of a multistep synthesis of PVA coated superparamagnetic nanoparti-cles,” J. Colloid Interface Sci., vol. 278, no. 2, pp. 353–360, 2004.  E. García-Matres, “Magnetic susceptibility and ¿eld-induced
transi-tions in R2BaNiO5 compounds ( , Er, Ho, Dy, Tb, Gd, Sm, Nd, Pr),” J. Magn. Magn. Mater., vol. 149, no. 3, pp. 363–372, 1995.  G. van Ewijk, “Convenient preparation methods for magnetic
col-loids,” J. Magn. Magn. Mater., vol. 201, no. 1–3, pp. 31–33, 1999.  D. A. Skoog, D. M. West, and F. J. Holler, Fundamentals of Analytical
Chemistry, 7th ed. Fort Worth, TX: Saunders College Pub., 1996.
 C. D. Muller and F. Schuber, “Fluorometric determination of polysty-rene latex: Application to the measurement of phagosomes and phago-cytosis,” Anal. Biochem., vol. 152, no. 1, pp. 167–171, 1986.  F. Timm, “Der histochemische Eisennachweis,” Histochemie, vol. 2,
no. 2, pp. 143–149, 1960.
 T. J. Brunner, P. Wick, P. Manser, P. Spohn, R. N. Grass, L. K. Lim-bach, A. Bruinink, and W. J. Stark, “In vitro cytotoxicity of oxide nanoparticles: Comparison to in vitro cytotoxicity of oxide,” Environ.
Sci. Technol., vol. 40, no. 14, pp. 4374–4381, 2006.
 H. Lee, E. Lee, D. K. Kim, N. K. Jang, Y. Y. Jeong, and S. Jon, “An-tibiofouling polymer-coated superparamagnetic iron oxide nanoparti-cles as potential magnetic resonance contrast agents for in vivo cancer imaging,” J. Amer. Chem.Soc., vol. 128, no. 22, pp. 7383–7389, 2006.
 M. Auffan, L. Decome, J. Rose, T. Orsiere, M. de Meo, V. Briois, C. Chaneac, L. Olivi, J.-L. Berge-Lefranc, A. Botta, M. R. Wiesner, and J.-Y. Bottero, “In vitro interactions between DMSA-coated maghemite nanoparticles and human ¿broblasts: A physicochemical and cyto-genotoxical study,” Environ. Sci. Technol., vol. 40, no. 14, pp. 4367–4373, 2006.
 A. Petri-Fink, B. Steitz, A. Finka, J. Salaklang, and H. Hofmann, “Ef-fect of cell media on polymer coated superparamagnetic iron oxide nanoparticles (SPIONs): Colloidal stability, cytotoxicity, and cellular uptake studies,” Eur. J. Pharm. Biopharm., vol. 68, no. 1, pp. 129–137, 2008.
 A. Vonarbourg, C. Passirani, P. Saulnier, and J.-P. Benoit, “Parameters inÀuencing the stealthiness of colloidal drug delivery systems,”
Bio-materials, vol. 27, no. 24, pp. 4356–4373, 2006.
 L. D. Galuppo, S. W. Kamau, B. Steitz, P. O. Hassa, M. Hilbe, L. Vaughan, S. Koch, A. Fink-Petri, M. Hofman, H. Hofman, M. O. Hot-tiger, and B. Rechenberg, “Gene expression in synovial membrane cells after intraarticular delivery of plasmid-linked superparamagnetic iron oxide particles—A preliminary study in sheep,” J. Nanosci.
Nan-otechnol., vol. 6, no. 9–10, pp. 2841–2852.
 M. Cournil and D. Di Benedetto, “Size analysis of ¿ne particle suspen-sions by spectral turbidimetry: Potential and limits,” Powder Technol., vol. 91, no. 3, pp. 197–208, 1997.
 S. D. Conner and S. L. Schmid, “Regulated portals of entry into the cell,” Nature, vol. 422, no. 6927, pp. 37–44, 2003.
 V. Stone, H. Johnston, and M. J. D. Clift, “Air pollution, ultra¿ne and nanoparticle toxicology: Cellular and molecular interactions,” IEEE
Trans. Nanobiosci., vol. 6, no. 4, pp. 331–340, Dec. 2007.
 A. Albanese and W. C. Chan, “Effect of gold nanoparticle aggregation on cell uptake and toxicity,” ACS Nano, vol. 5, no. 7, pp. 5478–5489, 2011.
 M. Mahmoudi, S. Laurent, M. A. Shokrgozar, and M. Hosseinkhani, “Toxicity evaluations of superparamagnetic iron oxide nanoparticles: Cell “vision” versus physicochemical properties of nanoparticles,”
ACS Nano, vol. 5, no. 9, pp. 7263–7276, 2011.